Theory of Multiband Superconductivity
Jun K
ONDO
*
AIST,Tsukuba Central 2,Tsukuba 3058568
(Received January 29,2002)
Superconductivity arising from coulomb repulsion between electrons has been studied for a multiband
system.We consider onsite and intersite coulomb integrals,intersite exchange integrals and intersite
exchangelike integrals [K of eq.(42)].We do not take account of the correlation eﬀect caused by the
interaction,such as spin ﬂuctuation etc.,and calculate the average of the interaction energy with the BCS
wave function.We ﬁnd that when K is so large that satisﬁes eq.(50),an stype superconducting state is
stable when there are two fermi surfaces.The gap functions on these fermi surfaces have diﬀerent signs
and so the pair transition between them gives us a negative energy for a positive K,leading to
superconductivity.
KEYWORDS:superconductivity,multiband,exchangelike integral,theory
DOI:10.1143/JPSJ.71.1353
1.Introduction
Superconductivity arising from coulomb repulsion has
been a subject of many theoretical works.A point of interest
for it is how a condensation energy (a negative energy)
arises from a positive interaction energy.
1,2)
The key is to
devide the kspace into two regions,where the sign of the
gap function is either positive or negative.The pair
transition from the positive region to the negative one or
the reverse transition gives us a negative energy,if the
matrix element of the transition is positive.When the k
dependence of the matrix element is appropriate,this
negative contribution overcomes the positive ones,which
arise from the pair transition within each region and results
in superconductivity.A bare coulomb repulsion incorporated
with the BCS wave function is not appropriate for this
scenario to be realized,and one must take the electron
correlation into the BCS wave function to obtain an eﬀective
interaction which has an appropriate kdependence
3–8)
or
take the correlation directly by using something like the
Gutzwiller projection.
9–11)
The aim to obtain a negative energy from a positive
interaction may also be achieved when one treats a twoband
or multiband superconductivity.In this case the sign of the
gap function within each band may be deﬁnite but diﬀerent
from each other.Then the pair transition between the bands
of diﬀerent signs of the gap may give us a negative energy
when the transition matrix element is positive.This scenario
was ﬁrst proposed by the present author
12)
and studied by
several authors for realistic substances.
13–22)
As we shall see
later,such a pair transition between bands is induced by an
exchanglike integral between atomic orbitals belonging to
diﬀerent bands.Our concern is that many other integrals,
such as onsite or intersite coulomb or exchange integrals,
might destroy the superconductivity caused by the interband
transition.This problem was not studied seriously in
previous works and we here present some results of the
study for the condition of realizing superconductivity from
the interband transiton.We consider a bipartite lattice and
ﬁrst ﬁnd a oneparticle eigenstate (Bloch orbitals) by
introducing intra and intersublattice transfer integrals.
Based on these Bloch states the interaction Hamiltonian is
expressed in terms of many integrals involving four atomic
orbitals.We keep only the onsite and intersite coulomb
integrals,the exchange and exchangelike integrals between
orbitals belonging to diﬀerent sublattices.With such a
Hamiltonian we take its average by the BCS wave function
extended to a multiband case.We do not take account of the
electron correlation,which means we work in the lowest
order of the interaction.Contrary to the single band case we
ﬁnd that superconductivity exists in a wide range of
reasonable parameter values without invoking higherorder
eﬀects of the interaction.In most cases superconductivity
exists when there are two fermi surfaces,on each of which
the sign of the gap function is deﬁnite but diﬀerent from
each other.In some cases the gap function may have zeros
even though it is essentially of the scharacter.
2.The Model
We consider L atomic orbitals in the unit cell denoted by
n
with ¼ 1; ;L.Here,n speciﬁes the unit cell,and the
position vector of the nth unit cell is denoted by R
n
and that
of the th atomic orbital measured from R
n
by
,so we
write as
n
ðrÞ ¼
ðr R
n
Þ:ð1Þ
Especially,we use the notation
0
¼
ðr
Þ.We
construct L LCAO’s from
n
as
u
k
¼
1
ﬃﬃﬃﬃ
N
p
X
n
e
ikR
n
n
;
ð2Þ
from which we obtain the eigenstates of the oneparticle
Hamiltonian as
k
l
¼
X
l
ðkÞu
k
l ¼ 1; ;L:
ð3Þ
Here N is the total number of the unit cells.The coeﬃcient
of the transformation,
l
ðkÞ,has the property
l
ðkÞ ¼
l
ðkÞ.
We now take account of the electronelectron interaction.
In the second quantization scheme,the electron ﬁeld is
described by
*
Correspondence should be addressed to 2229,Kamitakaido,Suginami
ku,Tokyo 1680074.
Journal of the Physical Society of Japan
Vol.71,No.5,May,2002,pp.1353–1359
#2002 The Physical Society of Japan
1353
ðr;Þ ¼
X
lk
a
lk
k
l
ðrÞ ðÞ;
ð4Þ
where denotes the spin coordinate and ðÞ is either the up
spin () function or the downspin (
) function.In this
scheme the interaction takes the form
H
0
¼
1
2
X
0
Z
y
ðr;Þ
y
ðr
0
;
0
ÞVðr;r
0
Þ ðr
0
;
0
Þ ðr;Þd d
0
:
ð5Þ
Among terms involved in eq.(5),we retain only those which
correspond to scattering of the Cooper pair.Thus we have
H
0
red
¼
1
2
X
lkl
0
k
0
V
lkl
0
k
0
X
0
a
y
lk
a
y
lk
0
a
l
0
k
0
0
a
l
0
k
0
;ð6Þ
where
V
lkl
0
k
0
¼ h
k
l
k
l
j
k
0
l
0
k
0
l
0
i:ð7Þ
In general we use the notation
h
i
j
j
l
k
i ¼
Z
i
ð1Þ
j
ð2ÞVð1;2Þ
l
ð1Þ
k
ð2Þd
1
d
2
:ð8Þ
The right hand side of eq.(7),which involves
k
l
’s,can be
expressed in terms of
n
’s by using eqs.(2) and (3).Among
integrals involving
n
’s,we retain only coulomb integrals,
exchange integrals and exchangelike integrals,whose
deﬁnitions will be shown presently.Thus we have
V
lkl
0
k
0
¼
1
N
X
n
0
e
iðkk
0
ÞR
n
l
ðkÞ
0
l
ðkÞ
l
0
ðk
0
Þ
0
l
0
ðk
0
Þh
0
n
0
j
0
n
0
i
þ
1
N
X
n
0
0
e
iðkþk
0
ÞR
n
l
ðkÞ
0
l
ðkÞ
0
l
0
ðk
0
Þ
l
0
ðk
0
Þh
0
n
0
j
n
0
0
i
þ
1
N
X
n
0
0
j
l
ðkÞj
2
j
0
l
0
ðk
0
Þj
2
h
0
0
j
n
0
n
0
i:ð9Þ
The integrals in each line of eq.(9) are,from the above,the coulomb integral,the exchange integral and the exchangelike
integral,respectively.All these integrals must be positive.The prime on the summation sign means to neglect the term with
n ¼ 0 and ¼
0
.We naturally have V
lkl
0
k
0
¼
VV
l
0
k
0
lk
.Furthermore we have V
lkl
0
k
0
¼ V
l
0
k
0
lk
,if the atomic orbitals are real,
which we assume to be the case.For simplicity we assume that all these atomic orbitals are of the stype.
Now we take the BCS wave function extended to a multiband case
¼
Y
lk
ðu
lk
þ
lk
a
y
lk"
a
y
lk#
Þj0i;
ð10Þ
and calculate the average of eq.(6) with it to ﬁnd
hH
0
red
i ¼
X
lkl
0
k
0
V
lkl
0
k
0
u
lk
lk
u
l
0
k
0
l
0
k
0
¼
1
N
X
n
0
h
0
n
0
j
0
n
0
i
X
lk
e
ikR
n
l
ðkÞ
0
l
ðkÞu
lk
lk
2
þ
1
N
X
n
0
0
h
0
n
0
j
n
0
0
i
X
lk
e
ikR
n
l
ðkÞ
0
l
ðkÞu
lk
lk
2
þ
1
N
X
n
0
0
h
0
0
j
n
0
n
0
i
X
lk
j
l
ðkÞj
2
u
lk
lk
X
lk
j
0
l
ðkÞj
2
u
lk
lk
:ð11Þ
The ﬁrst two terms,the coulomb term and the exchange
term,are positive deﬁnite and superconductivity is not
expected with only these terms,but the third therm,the
exchangelike term,may be negative and its negative
contribution to the energy may overcome the positive ones
of the ﬁrst two terms and result in superconductivity.We
will study the condition for this scenario to be realized.
Before starting calculation,we rewrite eq.(11) as
hH
0
red
i ¼ E
0
0
þ
1
N
X
n
0
0
½h
0
n
0
j
0
n
0
i þh
0
n
0
j
n
0
0
i
X
lk
e
ikR
n
l
ðkÞ
0
l
ðkÞu
lk
lk
2
;ð12Þ
where
E
0
0
¼ N
X
0
c
0
X
X
0
;ð13Þ
X
¼
1
N
X
lk
j
l
ðkÞj
2
u
lk
lk
;
c
0
¼
X
n
h
0
0
j
n
0
n
0
i ¼ c
0
:ð14Þ
In a simple and useful approximation,we keep only E
0
0
.It is
a quadratic form and will be indeﬁnite in sign when there is
at least one negative eigenvalue of the matrix c
0
.We will
later study this problem for a simple example.
Let"
lk
be the oneparticle energy of each band measured
1354 J.Phys.Soc.Jpn.,Vol.71,No.5,May,2002 J.K
ONDO
from the fermi level .(We consider the ground state of the
system.) Then the total energy with this energy included is
written as
E ¼ 2
X
lk
"
lk
2
lk
þ
X
lkl
0
k
0
V
lkl
0
k
0
u
lk
lk
u
l
0
k
0
l
0
k
0
:
ð15Þ
Minimization of this expression determines the variation
parameters u
lk
and
lk
as
u
2
lk
¼
1
2
1 þ
"
lk
E
lk
;ð16Þ
2
lk
¼
1
2
1
"
lk
E
lk
;ð17Þ
2u
lk
lk
¼
lk
E
lk
;ð18Þ
E
lk
¼
ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ
"
2
lk
þ
2
lk
q
;ð19Þ
with the selfconsistency equation
lk
¼
1
2
X
l
0
k
0
V
lkl
0
k
0
l
0
k
0
E
l
0
k
0
:
ð20Þ
We set
lk
¼ z
lk
,where represents the magnitude
of the gap ( > 0) and z
lk
its angular dependence.We
concentrate on the case of small ,when the following
relation holds
1,2)
X
k
FðkÞ
E
lk
¼ 2 log
X
k
FðkÞð"
lk
Þ
þðterms nondivergent as !0Þ:
Keeping only the ﬁrst contribution,we ﬁnd the self
consistency equation now reads
1
log
z
lk
¼
X
l
0
k
0
V
lkl
0
k
0
ð"
l
0
k
0
Þ z
l
0
k
0
:
ð21Þ
This is a homogenous linear equation with the eigenvalue
being 1= log .It is not an Hermitian equation and one
might wonder if the eigenvalue is real or not.That it is real
can be seen by multiplying both sides of eq.(21) by z
z
lk
ð"
lk
Þ
and summing over l and k:
1
log
X
lk
jz
lk
j
2
ð"
lk
Þ ¼
X
lkl
0
k
0
V
lkl
0
k
0
z
z
lk
z
l
0
k
0
ð"
lk
Þð"
l
0
k
0
Þ:
Since both sums are real and the one on the left hand side
does not vanish,we can conclude 1= log must be real.
Since we are restricting ourselves to the weak coupling limit,
a negative eigenvalue assures a superconducting ground
state.
We will obtain the expression for V
lkl
0
k
0
from eq.(11) or
eq.(12),but with E
0
0
we simply ﬁnd
V
lkl
0
k
0
¼
1
N
X
0
c
0
j
l
ðkÞj
2
j
0
l
0
ðk
0
Þj
2
:
ð22Þ
Hereafter we will tell about the results of keeping only E
0
0
,
but treatment of a more general case is straightforward and
the results of that case will be mentioned when it is
necessary.Since eq.(22) is the sum of the products of two
functions depending only on k and k
0
,the summation over k
0
in eq.(21) gives us a kindependent factor,which we denote
by x
:
x
¼
1
N
X
lk
j
l
ðkÞj
2
ð"
lk
Þz
lk
:
ð23Þ
Then eq.(21) reads
z
lk
¼
X
0
c
0
j
l
ðkÞj
2
x
0
:
ð24Þ
Insertion of this expression into eq.(23) gives us
x
¼
X
0
a
0
x
0
; ¼ 1; ;L ð25Þ
with
a
0
X
00
b
00
c
00
0
ð26Þ
and
b
0
1
N
X
lk
j
l
ðkÞj
2
j
0
l
ðkÞj
2
ð"
lk
Þ:ð27Þ
The dimension of the seqular equation has been reduced to
L.We note that b
0
involves only the band parameters,
whereas c
0
only the coulomb parameters.When eq.(25)
has a negative eigenvalue,we conclude that a super
conducting state is stable.The condition for a negative
eigenvalue is closely related to the condition that the matrix
c
0
has a negative eigenvalue and so E
0
0
is indeﬁnite.This
correlation is brought about by eq.(26).We will see an
example of this correlation in the next section.After solving
eq.(25) and ﬁnding x
within an arbitrary factor,we obtain
angular dependence of the gap function from eq.(24).
Without knowing details of the solution we see that the
symmetry of the gap function is a
1g
,because so is the
symmetry of j
l
ðkÞj
2
.
3.An Example of a Bipartite Square Lattice
As an example we consider a twodimensional two
sublattice model as shown in Fig.1,where L ¼ 2.The
LCAO’s on sublattice 1 and 2 are
u
k
1
¼
1
ﬃﬃﬃﬃ
N
p
X
n
e
ikR
n
1
ðr R
n
Þ;ð28Þ
u
k
2
¼
1
ﬃﬃﬃﬃ
N
p
X
n
e
ikR
n
2
ðr R
n
Þ;ð29Þ
Fig.1.Parameters of a twodimensional bipartite lattice.U
1
and U
2
are
onsite coulomb integrals and V
1
and V
2
are intersite coulomb integrals
on each sublattice,whereas t
1
and t
2
are transfer integrals in each
sublattice.V
0
,J and K are the coulomb,exchange and exchangelike
integrals between the sublattices.
J.Phys.Soc.Jpn.,Vol.71,No.5,May,2002 J.K
ONDO
1355
where ¼ ð1=2;1=2Þ.The lattice constant has been set to
unity.The one particle energy of these LCAO’s are
1k
¼ e
1
þ2t
1
ðcos k
x
þcos k
y
Þ ;ð30Þ
2k
¼ e
2
þ2t
2
ðcos k
x
þcos k
y
Þ ;ð31Þ
where t
1
and t
2
are the transfer integral in each sublattice and
e
1
and e
2
are the energy level of
1
and
2
,respectively.
We also consider transfer between nearest nighbouring
1
and
2
:
Z
uu
k
1
H
0
u
k
2
d ¼
0k
e
i’
k
;ð32Þ
0k
¼ 4t
0
cosðk
x
=2Þ cosðk
y
=2Þ;ð33Þ
’
k
¼ ðk
x
þk
y
Þ=2;ð34Þ
where t
0
is the relevant transfer integral (see Fig.1).
The eigenstates,eq.(3),are now expressed by
k
1
¼
1
1
ðkÞu
k
1
þ
2
1
ðkÞu
k
2
;ð35Þ
k
2
¼
1
2
ðkÞu
k
1
þ
2
2
ðkÞu
k
2
;ð36Þ
with
1
1
ðkÞ ¼ cos
k
;
2
1
ðkÞ ¼ e
i’
k
sin
k
;ð37Þ
1
2
ðkÞ ¼ e
i’
k
sin
k
;
2
2
ðkÞ ¼ cos
k
;ð38Þ
tan2
k
¼
0k
=
k
;
k
¼ ð
1k
2k
Þ=2;ð39Þ
whereas the eigenvalues by
"
1k
¼
1
2
ð
1k
þ
2k
Þ þ
ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ
ð
k
Þ
2
þ
2
0k
q
;ð40Þ
"
2k
¼
1
2
ð
1k
þ
2k
Þ
ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ
ð
k
Þ
2
þ
2
0k
q
:ð41Þ
From now on we retain only the following integrals and
equivalent ones:
U
1
¼ h
0
1
0
1
j
0
1
0
1
i;U
2
¼ h
0
2
0
2
j
0
2
0
2
i;
K ¼ h
0
1
0
1
j
0
2
0
2
i:
ð42Þ
We then have c
11
¼ U
1
,c
22
¼ U
2
,c
12
¼ c
21
¼ zK,where
z ¼ 4 is the number of the nearest neighbours.We also ﬁnd
from eqs.(26) and (27)
a
11
¼ b
11
U
1
þb
12
zK;a
12
¼ b
11
zK þb
12
U
2
;
a
21
¼ b
21
U
1
þb
22
zK;a
22
¼ b
21
zK þb
22
U
2
;ð43Þ
where
b
11
¼
1
N
X
k
½cos
4
k
ð"
1k
Þ þsin
4
k
ð"
2k
Þ;ð44Þ
b
22
¼
1
N
X
k
½sin
4
k
ð"
1k
Þ þcos
4
k
ð"
2k
Þ;ð45Þ
b
12
¼ b
21
¼
1
N
X
k
sin
2
k
cos
2
k
½ð"
1k
Þ þð"
2k
Þ:ð46Þ
From eq.(43) or eq.(26) one has
a
11
a
22
a
12
a
21
¼ BC;ð47Þ
where
C c
11
c
22
c
12
c
21
¼ U
1
U
2
ðzKÞ
2
;ð48Þ
B b
11
b
22
b
12
b
21
¼
1
N
2
X
kk
0
ðcos
2
k
sin
2
k
0
Þ
2
ð"
1k
Þð"
2k
0
Þ
þ
1
2N
2
X
kk
0
ðsin
2
k
sin
2
k
0
Þ
2
½ð"
1k
Þð"
1k
0
Þ þð"
2k
Þð"
2k
0
Þ 0:ð49Þ
When B > 0,the condition that eq.(25) has a negative eigenvalue,namely a
11
a
22
a
12
a
21
< 0,is equivalent to the
condition that the E
0
0
is indeﬁnite in sign,namely C < 0,or
ðzKÞ
2
U
1
U
2
> 0:
ð50Þ
On the other hand,when B ¼ 0,the smallest eigenvalue of eq.(25) is zero and so the superconducting state cannot be stable.
From eq.(49) we see that B ¼ 0 when (i) there exists only a single fermi surface and (ii) sin
2
k
is a constant on that surface.
This criterion is very useful for later arguments.The negative eigenvalue of eq.(25) is obtained for BC < 0 as
¼ ð1=2Þ
U
1
b
11
þU
2
b
22
þ2zKb
12
ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ
ðU
1
b
11
þU
2
b
22
þ2zKb
12
Þ
2
4BC
q
ð51Þ
When V
0
¼ h
0
1
0
2
j
0
1
0
2
i and J ¼ h
0
1
0
2
j
0
2
0
1
i are also kept,the second term of eq.(12) is found as
4ðV
0
þJÞ
N
"
X
k
cosðk
x
=2Þ cosðk
y
=2Þ sin 2
k
ðu
1k
1k
u
2k
2k
Þ
#
2
þ
4ðV
0
þJÞ
N
"
X
k
sinðk
x
=2Þ sinðk
y
=2Þ sin 2
k
ðu
1k
1k
u
2k
2k
Þ
#
2
ð52Þ
Here we naturally assumed that u
1k
1k
and u
2k
2k
have the same even or odd parity.When the symmetry of the gap function
is a
1g
,the second line vanishes,but the ﬁrst line does not because cosðk
x
=2Þ cosðk
y
=2Þ sin 2
k
is also of the a
1g
symmetry.
With the V
0
þJ term included we introduce
1356 J.Phys.Soc.Jpn.,Vol.71,No.5,May,2002 J.K
ONDO
1
¼
1
2N
X
k
cosðk
x
=2Þ cosðk
y
=2Þ sin 2
k
½z
1k
ð"
1k
Þz
2k
ð"
2k
Þ
beside x
1
and x
2
and solve the 3dimentional eigenvalue
problem.A term 4ðV
0
þJÞ cosðk
x
=2Þ cosðk
y
=2Þ sin 2
k
1
should be added to the right hand side of eq.(24) for
l ¼ 1 and subtracted from that for l ¼ 2.
4.Results
The results depend strongly on the band structure,which
is determined by t
0
,t
1
,t
2
,e
1
,e
2
.We discuss on two typical
cases of the band parameters.
4.1 Case 1:t
0
¼ 0:5,t
1
¼ 1,t
2
¼ 1,e
1
¼ 1,e
2
¼ 1
This is the case of two paralel and displaced dispersion
curves,which are repelled by the mixing t
0
between them.
The resulting dispersion"
1k
and"
2k
are shown in Fig.2.The
bands are partially ﬁlled when the fermi level is between
6:2 are 5.0.There are two fermi surfaces,when the fermi
level is between e
a
and e
b
of Fig.2.Outside of this there is
only a single fermi surface.
We have considered three cases for the choice of the
interaction parameters:
A:ðU
1
¼ 5;U
2
¼ 0:4;K ¼ 0:5Þ;
B:ðU
1
¼ 5;U
2
¼ 0:4;K ¼ 0:5;V
0
¼ 1;J ¼ 0:5Þ;
C:ðU
1
¼ 5;U
2
¼ 0:4;K ¼ 0:5;V
1
¼ 2;V
2
¼ 3;J ¼ 0:5Þ;
in all of which C ¼ 2.In Case C we consider the intersite
coulomb integrals in the same sublattice,V
1
and V
2
(see
Fig.1).Minus of the eigenvalue is shown in Fig.3,from
which we see that superconductivity exists only when the
fermi level is between e
a
and e
b
,namely only when there
exist two fermi surfaces.This is becasuse,outside of the
region between e
a
and e
b
,sin
2
k
is nearly constant on the
fermi surface and so the second term of eq.(49) vanishes
(the ﬁrst term naturally vanishes when there is only a single
fermi surface).The peaks at ¼ 1 and ¼ 1 are due to
the van Hove singularities.Cases B and C involve fairly
large coulomb integrals between sites,but still super
conductivity is robust around the van Hove singularity,if
C is not small (2 in this case).
We then discuss on the results of calculation of the gap
function based on eq.(24) or similar one including the
1
term.When the fermi level is between e
a
and 1:0 and not
close to the latter,the two fermi surfaces are nearly circular
and the gap functions are almost constant on them,but have
diﬀerent signs for the diﬀerent bands.This is what we
expected:diﬀerent signs of the gap function for the diﬀerent
bands and a positive scattering matrix element betwee them
give us a negative contribution to the interaction energy and
lead to superconductivity.We encounter a somewhat
diﬀerent situation near the van Hove singularity ¼ 1.
Fig.4 shows the fermi surfaces for the fermi level ¼ 1:1
and ¼ 0:9.A and C are those of the lower band and B
and D those of the upper band.Fig.5 shows the gap
functions on these fermi surfaces with an arbitrary scale for
Case B of the interaction parameters.One sees there are
Fig.2.The dispersion curves for case of t
0
¼ 0:5,t
1
¼ 1,t
2
¼ 1,
e
1
¼ 1,e
2
¼ 1 drawn from(0,0) to (;0) and from(0,0) to (;).When
the fermi level is between e
a
and e
b
,there exist two fermi surfaces.
Fig.3.Minus of the eigenvalue vs the fermi energy for the band
parameters of Fig.2 and the three choices of the interaction parameters
(see text).
Fig.4.The fermi surfaces for the dispersion curves of Fig.2 for the fermi
energy ¼ 1:1 and ¼ 0:9.The van Hove singularity is at
¼ 1:0.
Fig.5.The gap functions on Ato Din Fig.4 vs the angle between the k
x
axis and the radius vector drawn from (0,0) or (;).The interaction
parameters are Case B of §4.1.
J.Phys.Soc.Jpn.,Vol.71,No.5,May,2002 J.K
ONDO
1357
eight zeros of the gap on the larger fermi surface.This is also
the case for Case C but not the case for Case A,in which the
gap function is nearly constant even close to the van Hove
singularity.
4.2 Case 2:t
0
¼ 0:5,t
1
¼ 1,t
2
¼ 1,e
1
¼ 0,e
2
¼ 0
This is the case of the two crossing bands which are
mutually repelled by the mixing t
0
.The dispersion curves
are shown in Fig.6,from which one sees that in the regions
between ¼ 4:5 and 4 and between ¼ 4 and 4.5 there
exists only a single fermi surface.Figure 7 shows minus of
the eigenvalue for the three cases of the interaction
parameters as before.One ﬁnds that superconductivity does
not exist in the regions mentioned above for the same reason
as in §4.1.The van Hove singularities are at ¼ 0:97 and
¼ 0:97.When the fermi level is below 0:97,there are
two fermi surfaces,one centered at (0,0) and the other at
(;) (e.g.,A and B of Fig.8).The gap functions have a
constant sign on each of them,but have diﬀerent signs from
each other as in the case of §4.1.As the fermi level goes up
above 0:97,a crossover of the fermi surfaces results in C
and D surfaces of Fig.8.As one naturally sees from Fig.8,
each of the gap functions on C and D must have four zeros at
the four edges.The gap functions calculated based on eq.
(24) are shown in Fig.9 for the interaction parameters of
Case A.Results for Case B and Case C are similar.In the
parts of the fermi surfaces A and C of the ﬁgure,e.g.,which
are close to each other (denoted by+and+in Fig.8),the
values of the gap are almost the same.This is not apparent in
Fig.9,because the angle is not the same when the radius is
drawn from the center of A and from that of C to a point on
the fermi surface.
5.Discussion
We have seen an important role played by an exchange
like integral,such as h
0
0
j
n
0
n
0
i,in leading to multiband
superconductivity.Its eﬀect is enhanced by the factor z,the
number of the nearest neighbours of a bipartite lattice as is
seen in eq.(50).The negative eﬀect of the onsite coulomb
integrals is only cooperative,and if one of them is small,the
eﬀect is small even when the other is large.Thus the
presence of a weakly correlated band favours for the
superconductivity due to interband transition.Another point
of interest of eq.(50) is that z is larger in three dimension
and may be 6 at least.We may expect a more enhanced
eﬀect in three dimension.Superconductivity of MgB
2
may
be a candidate to treat along this scheme.
We have not taken account of the electron correlation
caused by the interaction.Thus the eigenvalue of the self
consistency equation is linear in the interaction parameters.
More precisely,when all the interaction parameters are
multiplied by and all the band parameters and the chemical
potential by ,the eigenvalue is multiplied by = .This is
easily seen in a special case,where only the parameter K is
Fig.6.The dispersion curves for case of t
0
¼ 0:5,t
1
¼ 1,t
2
¼ 1,
e
1
¼ 0,e
2
¼ 0,drawn from (0,0) to (;0) and from (0,0) to (;).When
the fermi level is between 4:5 and 4:0 or between 4.0 and 4.5,there
exists only a single fermi surface.
Fig.7.Minus of the eigenvalue vs the fermi energy for the band
parameters of Fig.6 and the same choices of the interaction parameters as
in §4.1.
Fig.9.The gap functions on Ato Din Fig.8 vs the angle between the k
x
axis and the radius vector drawn from (0,0),(;),(;0) or (0;).The
interaction parameters are Case A of §4.1.
Fig.8.The fermi surfaces for the dispersion curves of Fig.6 for the fermi
energy ¼ 1:0 and ¼ 0:93.The van Hove singularity is at
¼ 0:97 and ¼ 0:97.The gap functions are positive on A and
negative on B,but change signs on C and D.
1358 J.Phys.Soc.Jpn.,Vol.71,No.5,May,2002 J.K
ONDO
retained.From eq.(51) we then have
¼ zK
ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ
b
11
b
22
p
b
12
0
where b’s are inversely proportional to .
The symmetry of the gap function is a
1g
in the example of
§4,so is essentially of the scharacter.Then the eﬀect of the
onsite coulomb integrals is not suppressed,but super
conductivity still exists when inequality (50) is satisﬁed.
This is achieved by the gap function,which is positive in
some part of the fermi surface and negative in the other part
of it,while keeping the a
1g
symmetry.Such a gap function
takes advantage of the pair transition from the part of the
positive gap function to the part of the negative one.In most
cases such a gap function is realized when there are two
fermi surfaces,in one of which it is positive and in the other
it is negative.However it is also possible that the gap
function changes its sign on a single fermi surface with
several zeros,as we have seen in the example of §4.2.We
can expect that there are several types of the speciﬁc heat vs
temperature curve,when the present mechanism is relevant
to the superconductivity.
We have not taken account of the correlation between
electrons caused by the interaction.One of the important
consequences of this approximation is that it is not the
coulomb and exchange integrals but the exchangelike
integrals that are responsible for superconductivity.
Although this conclusion is quite general,the situation is
changed when one takes account of the correlation by a
perturbation theory or by a projection method.Even in this
case it is certain that the exchangelike integrals help to
enhance superconductivity.
1) J.Kondo:Bull.Electrotechnical Lab.(special issue) 64 (2000) 67.
2) J.Kondo:J.Phys.Soc.Jpn.70 (2001) 808.
3) W.Kohn and J.M.Luttinger:Phys.Rev.Lett.15 (1965) 524.
4) S.Nakajima:Prog.Theor.Phys.50 (1973) 1101.
5) P.W.Anderson and W.F.Brinkman:Phys.Rev.Lett.30 (1973) 1108.
6) K.Miyake,S.SchmittRink and C.M.Varma:Phys.Rev.B 34 (1986)
6554.
7) D.J.Scalapino,E.Loh,Jr.and J.E.Hirsh:Phys.Rev.B 34 (1986)
8190;ibid.35 (1987) 6694.
8) M.T.Be
´
alMonod,C.Bourbonnais and V.J.Emery:Phys.Rev.B 34
(1986) 7716.
9) T.Nakanishi,K.Yamaji and T.Yanagisawa:J.Phys.Soc.Jpn.66
(1997) 294.
10) K.Yamaji,T.Yanagisawa,T.Nakanishi and S.Koike:Physica C 304
(1998) 225.
11) K.Yamaji,T.Yanagisawa and S.Koike:Physica B 284–288 (2000)
415.
12) J.Kondo:Prog.Theor.Phys.29 (1963) 1.
13) P.Konsin,N.Kristoﬀel and T.O
¨
rd:Phys.Lett.A 129 (1988) 339.
14) P.Konsin and T.O
¨
rd:Physica C 191 (1992) 469.
15) B.K.Chakraverty:Phys.Rev.B 48 (1993) 4047.
16) K.Yamaji and Y.Shimoi:Physica C 222 (1994) 349.
17) K.Yamaji,Y.Shimoi and T.Yanagisawa:Physica C 235–240 (1994)
2221.
18) S.Koike,K.Yamaji and T.Yanagisawa:Physica C 282–287 (1997)
1765.
19) R.Combescot and X.Leyronas:Phys.Rev.Lett.75 (1995) 3732.
20) R.Combescot and X.Leyronas:Phys.Rev.B 54 (1996) 4320.
21) H.Nagao,M.Nishino,Y.Shigeta,Y.Yoshioka and K.Yamaguchi:J.
Chem.Phys.113 (2000) 11237.
22) H.Nagao,Y.Kitagawa,T.Kawakami,T.Yoshimoto,H.Sato and K.
Yamaguchi:Int.J.Quantum Chem.85 (2001) 608.
J.Phys.Soc.Jpn.,Vol.71,No.5,May,2002 J.K
ONDO
1359
Enter the password to open this PDF file:
File name:

File size:

Title:

Author:

Subject:

Keywords:

Creation Date:

Modification Date:

Creator:

PDF Producer:

PDF Version:

Page Count:

Preparing document for printing…
0%
Σχόλια 0
Συνδεθείτε για να κοινοποιήσετε σχόλιο